General

Property | Value | Condition | Shape |
---|---|---|---|

Density | 2.81 g/cm³ Show Material materials with Density of 2.81 g/cm³ | T73 | |

2.81 g/cm³ Show Material materials with Density of 2.81 g/cm³ | T73 | Bar | |

3.1 g/cm³ Show Material materials with Density of 3.1 g/cm³ | T73 |

Mechanical

Property | Temperature | Value | Condition | Shape | Related Standards | Comment |
---|---|---|---|---|---|---|

Compressive modulus | 72.4 MPa Show Material materials with Compressive modulus of 72.4 MPa | T73 | ||||

Elastic modulus | 72.0 GPa Show Material materials with Elastic modulus of 72.0 GPa | T73 | Bar | |||

Elongation | -195 °C | 14 % Show Material materials with Elongation of 14 % | T73 | Elongation in 50 mm | ||

-80 °C | 14 % Show Material materials with Elongation of 14 % | T73 | Elongation in 50 mm | |||

1.0 % Show Material materials with Elongation of 1.0 % | T73 | AA Standards, ASTM B247 | A100 | |||

2.0 % Show Material materials with Elongation of 2.0 % | T73 | AA Standards, ASTM B247 | A50 | |||

2.0 % Show Material materials with Elongation of 2.0 % | T73 | AA Standards, ASTM B247 | A100 | |||

3.0 % Show Material materials with Elongation of 3.0 % | T73 | AA Standards, ASTM B247 | A50 | |||

3.0 % Show Material materials with Elongation of 3.0 % | T73 | AA Standards, ASTM B247 | A100 | |||

5.0 % Show Material materials with Elongation of 5.0 % | T73 | AA Standards, ASTM B247 | A100 | |||

6.0 % Show Material materials with Elongation of 6.0 % | T73 | AA Standards, ASTM B221, ASTM B247 | A100 | |||

6.3 % Show Material materials with Elongation of 6.3 % | T73 | |||||

7.0 % Show Material materials with Elongation of 7.0 % | T73 | AA Standards, ASTM B221, ASTM B241, ASTM B247 | A50 | |||

7.0 % Show Material materials with Elongation of 7.0 % | T73 | AA Standards, ASTM B211, ASTM B221, ASTM B241 | A100 | |||

7.0 - 8.0 % Show Material materials with Elongation of 7.0 - 8.0 % | T73 | Bar | ||||

8.0 % Show Material materials with Elongation of 8.0 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241 | A50 | |||

9.0 % Show Material materials with Elongation of 9.0 % | T73 | AA Standards, ASTM B210, ASTM B211, ASTM B316 | A100 | |||

10.0 % Show Material materials with Elongation of 10.0 % | T73 | AA Standards, ASTM B210, ASTM B211 | A50 | |||

0 °C | 13 % Show Material materials with Elongation of 13 % | T73 | Elongation in 50 mm | |||

24 °C | 13 % Show Material materials with Elongation of 13 % | T73 | Elongation in 50 mm | |||

100 °C | 15 % Show Material materials with Elongation of 15 % | T73 | Elongation in 50 mm | |||

150 °C | 30 % Show Material materials with Elongation of 30 % | T73 | Elongation in 50 mm | |||

205 °C | 55 % Show Material materials with Elongation of 55 % | T73 | Elongation in 50 mm | |||

260 °C | 65 % Show Material materials with Elongation of 65 % | T73 | Elongation in 50 mm | |||

315 °C | 70 % Show Material materials with Elongation of 70 % | T73 | Elongation in 50 mm | |||

370 °C | 70 % Show Material materials with Elongation of 70 % | T73 | Elongation in 50 mm | |||

Fatigue strength | 159 MPa Show Material materials with Fatigue strength of 159 MPa | T73 | for 5x10⁸ cycles | |||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 7000 Series Aluminium | ||||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 7000 Series Aluminium | ||||

Shear modulus | 26.9 GPa Show Material materials with Shear modulus of 26.9 GPa | T73 | ||||

Tensile strength | -195 °C | 635 MPa Show Material materials with Tensile strength of 635 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

-80 °C | 545 MPa Show Material materials with Tensile strength of 545 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

395.0 MPa Show Material materials with Tensile strength of 395.0 MPa | T73 | AA Standards, ASTM B247 | ||||

400.0 MPa Show Material materials with Tensile strength of 400.0 MPa | T73 | AA Standards, ASTM B247 | ||||

405.0 MPa Show Material materials with Tensile strength of 405.0 MPa | T73 | AA Standards, ASTM B247 | ||||

415.0 MPa Show Material materials with Tensile strength of 415.0 MPa | T73 | AA Standards, ASTM B247 | ||||

420.0 MPa Show Material materials with Tensile strength of 420.0 MPa | T73 | AA Standards, ASTM B247 | ||||

425.0 MPa Show Material materials with Tensile strength of 425.0 MPa | T73 | AA Standards, ASTM B247 | ||||

435.0 MPa Show Material materials with Tensile strength of 435.0 MPa | T73 | AA Standards, ASTM B247 | ||||

440.0 MPa Show Material materials with Tensile strength of 440.0 MPa | T73 | AA Standards, ASTM B211, ASTM B247 | ||||

450.0 MPa Show Material materials with Tensile strength of 450.0 MPa | T73 | AA Standards, ASTM B221 | ||||

455.0 MPa Show Material materials with Tensile strength of 455.0 MPa | T73 | AA Standards, ASTM B210, ASTM B211, ASTM B247 | ||||

460.0 MPa Show Material materials with Tensile strength of 460.0 MPa | T73 | AA Standards, ASTM B209 | ||||

469.0 - 483.0 MPa Show Material materials with Tensile strength of 469.0 - 483.0 MPa | T73 | Bar | ||||

470.0 MPa Show Material materials with Tensile strength of 470.0 MPa | T73 | AA Standards, ASTM B211, ASTM B221, ASTM B241, ASTM B316 | ||||

475.0 MPa Show Material materials with Tensile strength of 475.0 MPa | T73 | AA Standards, ASTM B221, ASTM B241 | ||||

485.0 MPa Show Material materials with Tensile strength of 485.0 MPa | T73 | AA Standards, ASTM B221, ASTM B241 | ||||

500.0 MPa Show Material materials with Tensile strength of 500.0 MPa | T73 | |||||

0 °C | 525 MPa Show Material materials with Tensile strength of 525 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

24 °C | 503 MPa Show Material materials with Tensile strength of 503 MPa | T73 | ||||

100 °C | 435 MPa Show Material materials with Tensile strength of 435 MPa | T73 | ||||

150 °C | 215 MPa Show Material materials with Tensile strength of 215 MPa | T73 | ||||

205 °C | 110 MPa Show Material materials with Tensile strength of 110 MPa | T73 | ||||

260 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | T73 | ||||

315 °C | 55 MPa Show Material materials with Tensile strength of 55 MPa | T73 | ||||

370 °C | 40 MPa Show Material materials with Tensile strength of 40 MPa | T73 | ||||

Yield strength | -196 °C | 496 MPa Show Material materials with Yield strength of 496 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

-80 °C | 462 MPa Show Material materials with Yield strength of 462 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

-28 °C | 448 MPa Show Material materials with Yield strength of 448 MPa | T73 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

340.0 MPa Show Material materials with Yield strength of 340.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

345.0 MPa Show Material materials with Yield strength of 345.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

350.0 MPa Show Material materials with Yield strength of 350.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

360.0 MPa Show Material materials with Yield strength of 360.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

365.0 MPa Show Material materials with Yield strength of 365.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

370.0 MPa Show Material materials with Yield strength of 370.0 MPa | T73 | AA Standards, ASTM B247 | RP02 | |||

380.0 MPa Show Material materials with Yield strength of 380.0 MPa | T73 | AA Standards, ASTM B211, ASTM B221, ASTM B247 | RP02 | |||

385.0 MPa Show Material materials with Yield strength of 385.0 MPa | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B247, ASTM B316 | RP02 | |||

393.0 - 420.0 MPa Show Material materials with Yield strength of 393.0 - 420.0 MPa | T73 | Bar | RP02 | |||

395.0 MPa Show Material materials with Yield strength of 395.0 MPa | T73 | AA Standards, ASTM B221 | RP02 | |||

400.0 MPa Show Material materials with Yield strength of 400.0 MPa | T73 | AA Standards, ASTM B221, ASTM B241 | RP02 | |||

405.0 MPa Show Material materials with Yield strength of 405.0 MPa | T73 | AA Standards, ASTM B221, ASTM B241 | RP02 | |||

420.0 MPa Show Material materials with Yield strength of 420.0 MPa | T73 | AA Standards, ASTM B221, ASTM B241 | RP02 | |||

420.0 MPa Show Material materials with Yield strength of 420.0 MPa | T73 | |||||

425.0 MPa Show Material materials with Yield strength of 425.0 MPa | T73 | AA Standards, ASTM B211 | RP02 | |||

24 °C | 434 MPa Show Material materials with Yield strength of 434 MPa | T73 | ||||

100 °C | 400 MPa Show Material materials with Yield strength of 400 MPa | T73 | ||||

149 °C | 186 MPa Show Material materials with Yield strength of 186 MPa | T73 | ||||

204 °C | 90 MPa Show Material materials with Yield strength of 90 MPa | T73 | ||||

260 °C | 62 MPa Show Material materials with Yield strength of 62 MPa | T73 | ||||

316 °C | 45 MPa Show Material materials with Yield strength of 45 MPa | T73 | ||||

371 °C | 32 MPa Show Material materials with Yield strength of 32 MPa | T73 |

Thermal

Property | Value | Condition | Shape |
---|---|---|---|

Coefficient of thermal expansion | 2.3e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3e-05 1/K | T73 | |

2.35e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.35e-05 1/K | T73 | Bar | |

Melting point | 480.0 °C Show Material materials with Melting point of 480.0 °C | T73 | |

635.0 °C Show Material materials with Melting point of 635.0 °C | T73 | Bar | |

Specific heat capacity | 910.0 J/(kg·K) Show Material materials with Specific heat capacity of 910.0 J/(kg·K) | T73 | |

Thermal conductivity | 130.0 W/(m·K) Show Material materials with Thermal conductivity of 130.0 W/(m·K) | T73 | |

134.0 - 160.0 W/(m·K) Show Material materials with Thermal conductivity of 134.0 - 160.0 W/(m·K) | T73 | Bar |

Electrical

Property | Value | Condition | Shape | Comment |
---|---|---|---|---|

Electrical conductivity | 23000000 S/m Show Material materials with Electrical conductivity of 23000000 S/m | T73 | Typical/derived value | |

Electrical resistivity | 4.3099999999999996e-08 Ω·m Show Material materials with Electrical resistivity of 4.3099999999999996e-08 Ω·m | T73 | Typical value | |

4.31e-08 Ω·m Show Material materials with Electrical resistivity of 4.31e-08 Ω·m | T73 | Bar | ||

Specific Electrical conductivity | 40.0 % IACS Show Material materials with Specific Electrical conductivity of 40.0 % IACS | T73 | Typical value |

Chemical properties

Property | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|

Aluminium | 86.9 - 91.4 % Show Material materials with Aluminium of 86.9 - 91.4 % | T73 | |||

Chromium | 0.18 - 0.28 % Show Material materials with Chromium of 0.18 - 0.28 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Copper | 1.2 - 2.0 % Show Material materials with Copper of 1.2 - 2.0 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Iron | 0.50 % Show Material materials with Iron of 0.50 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | ||

0.5 % Show Material materials with Iron of 0.5 % | T73 | Bar | |||

Magnesium | 2.1 - 2.9 % Show Material materials with Magnesium of 2.1 - 2.9 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Manganese | 0.3 % Show Material materials with Manganese of 0.3 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Other | 0.15 % Show Material materials with Other of 0.15 % | T73 | Bar | Total | |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Titanium | 0.2 % Show Material materials with Titanium of 0.2 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Zinc | 5.1 - 6.1 % Show Material materials with Zinc of 5.1 - 6.1 % | T73 | AA Standards, ASTM B209, ASTM B210, ASTM B211, ASTM B221, ASTM B241, ASTM B247, ASTM B316 | Bar | |

Zirconium | 0.25 % Show Material materials with Zirconium of 0.25 % | T73 |

Technological properties

Property | ||
---|---|---|

Application areas | Aerospace | |

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: Operational damage in areas with tensile stresses transverse to the grain structure, limited damage to laboratory samples, general: good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (O), good to acceptable | |

Workability | general (condition): not suitable |